Effect of Sodium Fluoride Mouthwash on the Frictional Resistance of
Allahyar Geramy 1, Tabassom Hooshmand 2, Tahura Etezadi 3
1 Professor, Dental Research Center, Dentistry Research Institute, Tehran University of Medical Sciences, Tehran, Iran; Department of Orthodontics, School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran
2 Associate Professor, Department of Dental Materials, School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran 3 Assistant Professor, Department of Orthodontics, School of Dentistry, Mazandaran University of Medical Sciences, Sari, Iran
Objectives: The friction between the brackets and orthodontic wire during sliding mechanics inflicts difficulties such as decreasing the applied force and tooth movement and also the loss of anchorage. Therefore, many studies have focused on the factors that affect the friction. The purpose of this study was to assess the effect of 0.05% sodium fluoride mouthwash on the friction between orthodontic brackets and wire.
Materials and Methods: Four types of orthodontic wires including rectangular standard stainless steel (SS), titanium molybdenum alloy (TMA), nickel-titanium (NiTi) and copper-nickel-titanium (Cu-NiTi) were selected. In each group, half of the samples were immersed in 0.05% sodium fluoride mouthwash and the others were immersed in artificial saliva for 10 hours. An elastomeric ligature was used for ligating the wires to brackets. The frictional test was performed in a universal testing machine at the speed of 10 mm/minute. Two-way ANOVA was used for statistical analysis of the friction rate.
Results: The friction rate was significantly higher after immersion in 0.05% sodium fluoride mouthwash in comparison with artificial saliva (P=0.00). Cu-NiTi wire showed the highest friction value followed by TMA, NiTi and SS wires.
Conclusions: According to the results of the current study, 0.05% sodium fluoride mouthwash increased the frictional characteristics of all the evaluated orthodontic wires. Key words: Fluoride; Friction; Orthodontics; Saliva
Journal of Dentistry, Tehran University of Medical Sciences, Tehran, Iran (2017; Vol. 14, No. 5)
T. Etezadi, Department of Orthodontics, School of Dentistry, Mazandaran University of Medical Sciences, Sari, Iran
Received: 15 June 2017 Accepted: 10 August 2017
Sliding mechanics has gained increasing popularity among orthodontists. In this procedure, the wire slides through the brackets and tubes. The sliding resistance between the bracket slot and wire can influence tooth movement; therefore, control of friction during sliding mechanics is one of the most important factors for favorable treatment results [1-3]. The frictional force adversely affects the treatment process through decreasing or even inhibiting tooth movement, which can result in loss of anchorage. According to previous studies, the sliding friction reduces the applied force up to 50% [4-8]. Total elimination of this frictional
Fig. 1: The cling-shaped device used for holding the bracket during the upward movement of the superior jig of the testing machine
Since most orthodontic patients are adolescents who usually do not maintain a satisfactory oral hygiene, many clinicians recommend fluoride-containing products to patients [12-15]. The fluoride ion exerts a bactericidal effect by producing hydrofluoric acid (HF). Despite the suitable caries prevention effect of fluoride, production of HF can adversely affect orthodontic wires and brackets [10,13,16]. Previous investigations have shown that fluoride-containing products are destructive, especially for titanium-based alloys. The HF destroys the protective oxide layer on the appliance surface and causes corrosion [6,10,12,16]. The ions released due to corrosion can jeopardize the biocompatibility. Corrosion also alters the surface characteristics, which may lead to changes in the physical properties of the material with a subsequent influence on the clinical efficiency [6,14,17]. In a study by Kao et al , the orthodontic wires showed higher friction rates in the acidulated phosphate fluoride (APF) solution. To date, several studies have evaluated the effect of fluoride on the corrosion rate of orthodontic appliances, while investigation on the frictional resistance of wires after the use of fluoridated
products is limited, and no study has evaluated copper-nickel-titanium (Cu-NiTi) wires, which are used commonly in low-friction orthodontic treatment systems. The purpose of the present study was to assess the effect of 0.05% sodium fluoride mouthwash on the frictional resistance of different orthodontic wires.
MATERIALS AND METHODS
In the present study, 80 pieces of orthodontic wires of four different types were studied. The wires included stainless-steel (SS) alloy (Dentsply GAC International, NY, USA), titanium-molybdenum alloy (TMA) (Dentsply GAC International, NY, USA), super-elastic nickel-titanium (NiTi) alloy (Sentalloy, Dentsply GAC International, NY, USA) and copper-nickel-titanium (Cu-NiTi) alloy (Damon optimal-force Copper-NiTi, Ormco, Glendora, CA, USA).
The wires were rectangular and with the same dimensions of 0.018×0.025 inch2. Twenty pieces of
wire with the length of 5cm were used in each of the four groups. Eighty maxillary premolar stainless-steel standard edgewise brackets (American Orthodontics, Sheboygan, Wl, USA) with the slot size of 0.022 inch and without any torque or angulation were used for this study. All the wires and bracket slots were cleaned with alcohol wipes to remove manufacturing dirt and grease. Next, each group of wires was divided into 2 groups, as 10 pieces of each type of wire were placed in the test group and the other 10 pieces were employed in the control group. 0.05% sodium fluoride mouthwash with the pH of 6 (Oral-B, Procter and Gamble Strasse, Gross-Gerau, Germany) was used for evaluating the effect of fluoride. Artificial saliva with the pH of 6.5 was used as control with the following formulation: 2.2mM calcium chloride (CaCl2), 2.2mM
monosodium phosphate (NaH2PO4), 50mM
acetic acid, 100mM sodium chloride (NaCl), 1 part per million (ppm) sodium fluoride (NaF), and 0.02% sodium azide (NaN3). The samples in
Table 1. Mean and standard deviation (SD) of the frictional force (N) related to four types of wires in two different environments
SS TMA NiTi Cu-NiTi
0.05% Sodium fluoride mouthwash
1.36±0.18 1.63±0.15 1.45±0.04 1.77±0.23
saliva 1.14±0.24 1.47±0.14 1.36±0.31 1.64±0.26
SS=Stainless Steel, TMA=Titanium Molybdenum Alloy, NiTi=Nickel-Titanium, Cu-NiTi=Copper-Nickel-Titanium
hours (10 wires were placed in artificial saliva, while the other 10 wires were immersed in fluoride-containing mouthwash). Afterwards, the samples were placed in an incubator at 37°C. After 10 hours, the samples were immersed in distilled water for 30 minutes. In order to exclude the influence of different elastomeric forces on the results, an elastomeric ligature (American Orthodontics, Sheboygan, Wl, USA) was used to engage the dried wires with brackets by using a special gun type elastomeric ring placer (Hangzhou Sino Ortho Technology Co., Ltd., China). The frictional test was performed in a universal testing machine (Zwick/Roell Z050, Germany). A special fixture and a rigid cling-shaped device (to grab the bracket during the frictional test) were designed and fabricated. The fixture was attached to the inferior jig of the testing machine to fix the wire. Next, the bracket was moved upwards along the 5-mm stretch of wire by the cling-shaped device attached to the superior jig of the machine (Fig. 1) at the speed of 10 mm/minute . Care was taken to align the wire with a completely straight direction during bracket-sliding. The force required to initiate and maintain the bracket movement over the 5-mm test distance was measured. The program was set to highlight the maximum frictional force. Two-way ANOVA was used to compare the friction rate related to the tested solutions and also between the four types of
wires. Bonferroni correction was applied as a post-hoc test. The level of significance was set at P<0.05.
Table 1 shows the frictional force values of the groups categorized by the two different environments of sodium fluoride mouthwash and artificial saliva. According to two-way ANOVA, the frictional force of all the samples significantly increased after immersion in sodium fluoride solution (P=0.00). Different friction values were obtained in the four groups of wires. In both environments (saliva and fluoride solution), Cu-NiTi wire exhibited the highest friction values followed by TMA, NiTi and SS wires. The differences between the frictional forces of different wire types were analyzed by Bonferroni's test. As shown in Table 2, there were statistically significant differences between SS group and Cu-NiTi and TMA groups (P=0.00), and also between Cu-NiTi and NiTi wires (P=0.00).
Table 2. Comparison of the frictional force (N) between the four groups of wires
Wire type Mean
TMA -0.29* 0.07 0<001*
NiTi -0.15 0.07 0.15
Cu-NiTi -0.45* 0.07 0<001*
SS 0.29* 0.07 0<001*
NiTi 0.14 0.07 0.21
Cu-NiTi -0.16 0.07 0.12
SS 0.15 0.07 0.15
TMA -0.14 0.07 0.21
Cu-NiTi -.30* 0.07 0<001*
SS 0.45* 0.07 0<001*
TMA 0.16 0.07 0.12
NiTi 0.30* 0.07 0<001*
SS=Stainless Steel, TMA=Titanium Molybdenum Alloy, NiTi=Nickel-Titanium, Cu-NiTi=Copper-Nickel-Titanium
in the APF solution. In another similar study by Nanjundan and Vimala , fluoride mouthwash raised the frictional resistance of SS wires, which is consistent with our results. However, Alavi and Farahi  revealed different results. They reported that the friction rates of SS and NiTi wires were higher in the fluoride gel with a high fluoride concentration, but no difference was observed between the fluoride mouthwash with a low fluoride content and the control group. The duration of immersion in the mentioned study was shorter than that in our study (2 minutes per day for two weeks), which makes it difficult to compare the results of the two studies. Abbassy  demonstrated that fluoride application does not significantly change the frictional resistance of SS and NiTi wires. This study also used shorter immersion time than ours (1 hour). To date, no other research has evaluated the effect of fluoride on Cu-NiTi wires. In the present experiment, daily sodium fluoride mouthwash increased the frictional resistance of this type of
wire, which is commonly used in the self-ligating mechanics. This might have an adverse effect on the self-ligating mechanics, which is known as a low-friction system.
Comparison of the friction rate between four types of wires revealed that Cu-NiTi showed the highest frictional resistance in saliva and sodium fluoride solution, followed by TMA, NiTi and SS wires. This result is in agreement with the findings of previous studies. In a research by Kapila et al , round and rectangular TMA wires showed the highest rate of frictional resistance followed by NiTi, whereas SS wire exhibited the lowest amount of frictional resistance. Kao et al  also reported that the friction values decreased in TMA, NiTi and SS wires, respectively. Similarly, Fidalgo et al  showed that TMA wires have higher frictional resistance than SS wires, irrespective of the bracket system. Further evaluation of Cu-NiTi wires is recommended. The present study has some limitations that should be taken into consideration when interpreting the data. The duration of fluoride application may influence its effect on the wire characteristics. Also, it is difficult to exactly simulate the oral environment. Overall, this study showed that fluoride can raise the friction level during the sliding mechanics, which is worth considering, as it may negatively affect tooth movement, anchorage and treatment results. Further in-vivo investigations are needed to evaluate the precise effect of fluoride on orthodontic wires.
We would like to acknowledge the staff at dental research center of Tehran University of Medical Sciences for helping us to work with testing machine. We are especially grateful to DR. AR. Shamshiri for doing statistical test of the study (grant No:757).
1- Bandeira AM, dos Santos MP, Pulitini G, Elias CN, da Costa MF. Influence of thermal or chemical degradation on the frictional force of an experimental coated NiTi wire. Angle Orthod. 2011 May;81(3):484-9. 2- Fidalgo TK, Pithon MM, Maciel JV, Bolognese AM. Friction between different wire bracket combinations in artificial saliva--an in vitro evaluation. J Appl Oral Sci. 2011 Jan-Feb;19(1):57-62.
3- Tecco S, Tete S, Festa F. Friction between archwires of different sizes, cross-section and alloy and brackets ligated with low-friction or conventional ligatures. Angle Orthod. 2009 Jan;79(1):111-6.
4- Wichelhaus A, Geserick M, Hibst R, Sander FG. The effect of surface treatment and clinical use on friction in NiTi orthodontic wires. Dent Mater. 2005 Oct;21(10):938-45.
5- Kusy RP, Whitley JQ, Mayhew MJ, Buckthal JE. Surface roughness of orthodontic archwires via laser spectroscopy. Angle Orthod. 1988 Jan;58(1):33-45. 6- Huang HH. Variation in surface topography of different NiTi orthodontic archwires in various commercial fluoride-containing environments. Dent Mater. 2007 Jan;23(1):24-33.
7- Kapila S, Angolkar PV, Duncanson MG Jr, Nanda RS. Evaluation of friction between edgewise stainless steel brackets and orthodontic wires of four alloys. Am J Orthod Dentofacial Orthop. 1990 Aug;98(2): 117-26. 8- Husmann P, Bourauel C, Wessinger M, Jager A. The frictional behavior of coated guiding archwires. J Orofac Orthop. 2002 May;63(3):199-211.
9- Clocheret K, Willems G, Carels C, Celis JP. Dynamic frictional behaviour of orthodontic archwires and brackets. Eur J Orthod. 2004 Apr;26(2):163-70.
10- Kao CT, Ding SJ, Wang CK, He H, Chou MY, Huang TH. Comparison of frictional resistance after immersion of metal brackets and orthodontic wires in a fluoride-containing prophylactic agent. Am J Orthod Dentofacial Orthop. 2006 Nov;130(5): 568.e1-9.
11- Prashant PS, Nandan H, Gopalakrishnan M. Friction in orthodontics. J Pharm Bioallied Sci. 2015 Aug;7(Suppl 2):S334-8.
12- Walker MP, White RJ, Kula KS. Effect of fluoride prophylactic agents on the mechanical properties of nickel-titanium-based orthodontic wires. Am J Orthod Dentofacial Orthop. 2005 Jun;127(6):662-9.
13- Kwon YH, Jang CM, Jang JH, Park JH, Kim TH, Kim HI. Effect of fluoride released from fluoride-containing dental restoratives on NiTi orthodontic wires. Dent Mater J. 2008 Jan;27(1):133-8.
14- Schiff N, Grosgogeat B, Lissac M, Dalard F. Influence of fluoridated mouthwashes on corrosion resistance of orthodontics wires. Biomaterials. 2004;25(19):4535-42.
15- Li X, Wang J, Han E, Ke W. Influence of fluoride and chloride on corrosion behavior of NiTi orthodontic wires. Acta Biomater. 2007;3(5):807-15. 16- Kwon YH, Cho HS, Noh DJ, Kim HI, Kim KH. Evaluation of the effect of fluoride‐containing acetic acid on NiTi wires. J Biomed Mater Res B Appl Biomater. 2005 Jan;72(1):102-8.
17- Suarez C, Vilar T, Gil J, Sevilla P. In vitro evaluation of surface topographic changes and nickel release of lingual orthodontic archwires. J Mater Sci Mater Med. 2010 Feb;21(2):675-83.
18- Nanjundan K, Vimala G. Evaluation of frictional resistance and surface characteristics after immersion of orthodontic brackets and wire in different chemical solutions: A comparative in vitro study. Indian J Dent Res. 2016 Sep-Oct;27(5):513-520.
19- Alavi S, Farahi A. Effect of fluoride on friction between bracket and wire. Dent Res J (Isfahan). 2011 Dec;8(Suppl 1):S37-42.